Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Nanoscale Advances View Article Online REVIEW Cite this: DOI: 10.1039/d0na00590h View Journal Advances in the electron diﬀraction characterization of atomic clusters and nanoparticles Arturo Ponce, a Jeﬀery A. Aguilar, bc Jess Tated and Miguel José Yacamán*e Nanoparticles and metallic clusters continue to make a remarkable impact on novel and emerging Received 20th July 2020 Accepted 15th November 2020 technologies. In recent years, there have been impressive advances in the controlled synthesis of clusters and their advanced characterization. One of the most common ways to determine the DOI: 10.1039/d0na00590h structures of nanoparticles and clusters is by means of X-ray diﬀraction methods. However, this requires the clusters to crystallize in a similar way to those used in protein studies, which is not possible in many rsc.li/nanoscale-advances cases. Novel methods based on electron diﬀraction have been used to eﬃciently study individual nanoparticles and clusters and these can overcome the obstacles commonly encountered during X-ray a Department of Physics and Astronomy, The University of Texas at San Antonio, San Antonio, Texas 78249, USA d University of Utah, Scientic Computing Imaging Institute, Department of Electrical and Computer Engineering, Salt Lake City, Utah, USA b e Idaho National Laboratory, Nuclear Science and Technology Division, Idaho Falls, Idaho, 83415, USA c Lockheed Martin Space, Advanced Technology Center, Palo Alto, California, 94304, USA Arturo Ponce is an Associate Professor and Associate Chair in the Department of Physics and Astronomy at the University of Texas at San Antonio. He leads the Structure Physics and Electron Microscopy group at UTSA. He received his PhD in Materials Science from the University of Cadiz, Spain, and worked as a postdoctoral researcher at UNAM, Mexico, and CNRS, France. His research spans the theoretical and experimental aspects of the atomic structures, physical properties, and manipulation of materials on the nanoscale based on electron–matter interaction phenomena such as electron diﬀraction, electron holography, electron dose-controlled, and in situ microscopy. This journal is © The Royal Society of Chemistry 2020 Department of Applied Physics and Materials Science and Center for Materials Interfaces in Research and Applications, Northern Arizona University, Flagstaﬀ, AZ, USA. E-mail: [email protected] Jeﬀery A. Aguiar is a recognized expert in materials engineering, analytical instrumentation, and intelligence and materials research spanning global and nationwide collaborations, including in premier national research facilities at national laboratories, in universities, and in industry. He possesses expert knowledge of ultra-high temperature radiation hardened energy materials, characterization, and informatics-based approaches. Prior roles include being an invited academic faculty member at the University of Utah and technical deputy director of the Nuclear Materials Discovery and Qualication Initiative at Idaho National Laboratory. Now a senior scientist at Lockheed Martin's Advanced Technology Center with a diverse group of researchers and technical staﬀ, he focuses on advances in ultra-high strength materials and novel concepts to enable future space missions. Aguiar is a professional author of more than 50 peer-reviewed publications and technical contributions, and a professional committee member of the Materials Research Society. In addition, he is a recipient of the Idaho National Laboratory's prestigious early career award recognized for his expertise in materials, with ve patents, including an innovative approach to materials discovery using deep learning. Nanoscale Adv. View Article Online Nanoscale Advances Review diﬀraction methods without the need for large crystals. These novel methodologies have improved with Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. advances in electron microscopy instrumentation and electron detection. Here, we review advanced methodologies for characterizing metallic nanoparticles and clusters using a variety of electron diﬀraction procedures. These include selected area electron diﬀraction, nanobeam diﬀraction, coherent electron diﬀraction, precession electron diﬀraction, scanning transmission electron microcopy diﬀraction, and high throughput data analytics, which leverage deep learning to reduce the propensity for data errors and translate nanometer and atomic scale measurements into material data. Introduction One of the most active elds in nanotechnology is related to the synthesis and characterization of metallic conned nanostructures, such as nanoparticles and clusters. The precise control of the size and shape of such nanostructures is challenging. Traditionally, when a nanoparticle has a relatively small number of atoms it is referred to as a cluster, these are more prone to grow in a controlled atomic way with a very precise number of atoms.1–5 In recent years there has been impressive advances in the controlled synthesis of clusters.6–10 This has resulted in a new eld named atomically precise chemistry. Even though the boundary between clusters and nanoparticles is not precisely known, a cluster size ranges from 1 to 2 nm with perhaps no more than 500 atoms. Two examples of metallic clusters are shown in Fig. 1a and b obtained by aberration-corrected scanning transmission electron microscopy (Cs-STEM). As the number of atoms increases the properties change. To understand the properties, it is necessary to know the structure of the cluster. The most extended method used is X-ray diﬀraction. Starting from the determination of the Jess Tate received his PhD in Bioengineering from the University of Utah. His experience in computational modeling, image processing, and soware engineering carried over into material science research focused on improving the real-time processing of microscopy data. He is currently a Research Associate at the Scientic Computing and Imaging Institute. Nanoscale Adv. Au102 cluster11 several other clusters have been determined, such as Au25(SR)18, Au38(SR)24 (SR ¼ cyclohexylthiol), Au30(S-tBu) and many others.12–14 The main diﬃculty in X-ray diﬀraction is the need for the single crystal to be reliable. That means that a supercrystal of clusters must be generated. This is not possible for all clusters and this is the main limitation of the technique. Additionally, X-ray diﬀraction is a technique in which averages over a large area and local cluster variations cannot be observed. Electron diﬀraction, on the other hand, is a local technique that can be used to determine the structure of individual clusters and nanoparticles. In this review we will discuss the methods of electron diﬀraction and will show that it has the same eﬀectivity as X-ray diﬀraction and could become the most utilized technique for studying clusters and nanoparticles. X-ray diﬀraction is produced by single scattering events (kinematical scattering). Electrons on the other hand interact with matter 104 times more than X-ray diﬀraction. Therefore, electron diﬀraction patterns contain a lot more information. However, a complication arises from the multiple scattering events that are present in electron diﬀraction, leading to Miguel José Yacamán received his Bachelor's and Master's degrees in Physics, and a Ph.D. in Materials Science from the Universidad Nacional Autónoma de Mexico (UNAM), and performed postdoctoral work at the University of Oxford and at NASA-AMES Research Center in California. He has received Honoris Causa Doctorates from the Universidad Autónoma de Nuevo León and from the Universidad Nacional de Córdoba. He is currently a Professor at the Applied Physics and Materials Science Department of Northern Arizona University. He has supervised about 125 students and more than 100 post-doctoral researchers. He is fellow of the MRS, AVS, APS, MSA, and AAAS. He has more than 500 publications, and a h-index factor of 73. He has been awarded the National Prize in Exact Sciences from the Mexican Academy of Sciences, National Prize of Sciences in México, the John Weatley Award of the American Physical Society, the Exact Sciences Prize from the State of México, the Melh Award and the Distinguished Lecture of the U.S. Metals and Materials Society, and a Guggenheim Fellowship, among others. This journal is © The Royal Society of Chemistry 2020 View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Review Examples of gold cluster structures: (a) decahedron and (b) icosahedron. Fig. 1 dynamical eﬀects. In the electron–matter interactions, shown in Fig. 2, k and k0 , the incident and diﬀracted wavevectors satisfy the Laue condition. The diﬀerence vector k k' ¼ G, is the change owing to diﬀraction and represents an arbitrary point in the reciprocal space. The scattered beam satises the Bragg condition as |k| ¼ |k'| ¼ 2p/l, with l representing the wavelength. The multiple diﬀractions shown in Fig. 2 can fall into the allowed and forbidden ghkl positions, which are not allowed using the extinction rules calculated from the structure factor and makes elucidation of the crystal diﬃcult, even for very thin crystals.15 The result is that the intensity of the spots is not equal to Fh2, in which Fh is the structure factor.15,16 In the case of a large diﬀraction this can be overcome using precession diﬀraction,17 as we will discuss in the following sections. However, for the case of a metallic cluster, with only a limited number of atoms, the situation is more complicated because the atomic arrays are not necessarily located in conventional crystallographic directions. Fig. 3 shows the atomic planes on the cluster Au146 as reported by Vergara et al.18,19 Fig. 3a is oriented along the  0] direction (both direction and Fig. 3b is oriented along the [11 Nanoscale Advances Fig. 3 Atomic order in two low index directions (in fcc notation) for the cluster Au144 (a) along the  direction and (b) view along the  direction view along the atomic distribution “seen” by the electron beam is not one of atomic columns oriented in an ordered manner. This will result in a complicated electron diﬀraction pattern.19 shown as fcc directions). As can be seen, the atoms are not aligned in well-dened columns projected along both directions (some of them are indicated by the arrows). In this way, electrons traveling through a cluster will suﬀer multiple scatterings and will register these small atomic variations. The resulting diﬀraction pattern is directly related to the cluster structure. This can also be rephrased, meaning that the Bragg law cannot be used in the case of clusters. The Bragg law requires scattering in at least 10 atomic rows in order to produce coherent interference of the electron waves. As the number of atoms increases the diﬀraction pattern will become more dened. In the case of nanoparticles that are greater than 5 nm in size, the diﬀraction pattern already shows features as size streaks which are well known for bulk crystals. Despite the diﬃculties it is possible to calculate the diﬀraction pattern of clusters considering a structural model and using a modied version of the multislice method,20 which does not require atomic potential periodicity. An important aspect to be emphasized is that X-ray diﬀraction implies an average of all the present structures; therefore, individual variations are lost. Even with the best separation methods available it cannot be assumed that all the clusters are identical. On the other hand, electron diﬀraction is a localized technique and if the spot size is controlled it is possible to obtain individual cluster patterns and test for structural variations. If the clusters are placed on a carbon grid for transmission electron microscopy (TEM) examination, 108 nanoparticles per cm2 are typically and estimated to be present. It is possible to obtain a huge amount of data, which allows researchers to employ machine learning methods for structural determination by using a database of the crystallographic information. Radiation damage Fig. 2 Multiple scattering events during electron diﬀraction. This journal is © The Royal Society of Chemistry 2020 Clusters and nanoparticles are very sensitive to radiation damage caused by the electron beam. To successfully study clusters and nanoparticles radiation damage must be controlled. The main mechanisms of radiation damage in protected metallic clusters are: (i) radiolysis, (ii) knock on eﬀect of surface atoms, and (iii) the Auger eﬀect.21 Radiolysis aﬀects lighter atoms, for example ligands used to stabilize clusters, Nanoscale Adv. View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Nanoscale Advances and the accelerating voltage is not the primary radiation damage. When the number of atoms is large, such as in 50 nm particles, the knock on eﬀect of bulk atoms becomes important and the reduction of the accelerating voltage prevents the damage. Therefore, in each case we must nd a compromise acceleration voltage to minimize the overall damage. Radiolysis can be recognized because carbon molecules from the ligand redeposit on the cluster and form a halo that blurs the image. The number of atoms in the nth shell of an icosahedron can be obtained by 10n2 + 2, here n is the cluster number. A common metal cluster is the 13-atom icosahedron (n ¼ 1). The structure has one central atom and 12 surrounding atoms, 20 faces, 12 vertices and 30 edges. For subsequent numbers, the number of atoms adopts the form ni ¼ ni1 + (ni2 + 2); for example, n4 ¼ 147 + (42 + 2) ¼ 309. The sequence shown in Fig. 4 illustrates the cluster number and the estimated diameter, for cluster n ¼ 21 one will obtain 33 153 atoms and a nanoparticle of 11.504 nm, the structures were modeled in VESTA soware.22 The transition from a cluster to a nanoparticle occurs when a plasmonic eﬀect starts to appear. Clusters exhibit quantized properties as the quantum eﬀects are dominant, this denes the unique properties of the specic cluster number. Clusters are unstable without the protection of their surfaces, which is given by ligands attached to their surfaces. For instance, the Au144(thiolate)60 cluster is stabilized by a thiolate group, 2 phenylethanethiolate.23 Beam sensitive samples, such as organic materials or ligand protected metallic clusters, require a much lower dose of electron beam radiation to avoid damaging the sample.24 There have been many developments that have improved the high resolution of microscopes at low dose congurations. One of these is the introduction of highly sensitive sensors, which allows the detection of single electron events.25,26 Low dose beam radiation can also be used in addition to other techniques that allow a wide range of new information that can be attained from the specimen. Electron diﬀraction methods at low dose congurations are another alternative to obtain the crystallography of biological and sensitive samples. Another methodology is phase retrieval in electron holography at low doses as Review a systematic approach to reduce the electron beam current in the sample.27–29 Detection is a very important aspect in low dose radiation and illumination cannot be visualized with binoculars using low doses. According to Buban, et al.,30 catalysts are believed to cause damage at the order of 100 e Å2, biological samples with sugar embedded specimens require doses of <20 e Å2, and biological samples kept under liquid nitrogen require doses of <5 e Å2. Many of these advances enabled progress in the methods used for increasing the high-resolution imaging methods using low dose congurations. For STEM, using a probe-corrected microscope, the diameter of the electron beam (1.0 A) can resolve individual columns, but the current density increases substantially and deteriorates sensitive materials, such as the protected ligands of the clusters. To measure the number of electrons interacting with the specimen, one needs to use a Faraday cup to collect the electric current produced by the electron beam, which is an accurate device used to measure the electric current in the specimen region. Fig. 5a shows the experimental set up of the Faraday cup attached to a JEOL 2010F microscope and Fig. 5b shows an image of the electron beam collected at a magnication of 800 K using a complementary metal oxide semiconductor (CMOS) camera (TVIPS). When the Faraday cup is employed the number of electrons per area can be directly estimated. However, if the current density is measured on the screen the magnication must be considered, for example pA cm2 (1 A ¼ 1 C s1 ¼ 6.24 1018 electrons per s). Fig. 5b was collected using the minimum illumination possible by forcing the condenser lens (a) Experimental set-up of the Faraday cup device used to measure the electric current of the electron beam. (b) An electron beam probe registered at a magniﬁcation of 800 K, and (c) the intensity proﬁle of an electron beam probe with a diameter of approximately 55 nm. Fig. 5 Fig. 4 Atomic models of the icosahedral metal cluster and nanoparticles for diﬀerent values of n (1, 2, 3, 4, 6, 14, 19, and 21) and the total number of atoms upon growing the cluster to the nth shell. Nanoscale Adv. This journal is © The Royal Society of Chemistry 2020 View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Review voltage up to 8.06 V, the diameter of the region of illumination is shown in the intensity prole shown in Fig. 5c. In the microscope used, the current registered using the ammeter was 35 pA (diameter of the beam 55 nm), which corresponds to 920 electrons per A2 per second. When the number of electrons is measured using the screen plate of the microscope (2.2 pA cm2 at a magnication of 800 K times, 880 electrons per A2 are registered), the number of electrons is about 40 electrons per A2 less than the value obtained using the Faraday cup. The conversion used for the calculation is:31 2.2 pA cm2 6 241 500 e pA1 1 s per frame 1 1016 cm2 Å2 800 0002 ¼ 878 e Å2 s1 If the same current density is shown on the screen, but the diameter is reduced to 2.5 nm, the number of electrons is about two orders of magnitude higher (4.4 105 electrons per A2 per s). The current density can also be modied using diﬀerent apertures of the condenser lens. Using STEM, the current density increases exponentially. Current densities measured using a JEOL ARM200F with a probe corrector are shown in Fig. 6a. The electric current values were obtained using the same Faraday cup as previously described. The aperture of the condenser lens used was set to 20 mm and the extraction voltage A2 was held constant. The curve shown in Fig. 6a was obtained by reducing the extraction voltage A1. The images shown in Fig. 6a–e were recorded using a high angle annular dark eld detector (HAADF) in the STEM mode using standard emission in the microscope (A1 ¼ 3.14 kV, A2 ¼ 7.05 kV and a current measured of 4.9 pA). The HAADF-STEM images correspond to gold clusters of approximately 3.8 nm (Fig. 6b) and approximately 1.6 nm (Fig. 6d), both ligandprotected. When the eld of view is reduced to approximately 9 9 nm, the bigger cluster is more stable to the electron dose (Fig. 6c), while the smaller cluster deteriorates (Fig. 6e). Using the currents measured for standard emission and a probe size of around 1 A, the electron dose is approximately 4 107 elec2 trons per A . The electron dose measured from the curve in Fig. 6 (a) Electron current versus extraction voltage in a JEOL ARM200F operated at 200 kV. HAADF-STEM images of gold thiolate protected clusters of approximately 3.8 nm at (b) medium magniﬁcation and (c) high resolution. Images of approximately 1.6 nm clusters at (d) medium magniﬁcation, and (e) an example of radiation damage in gold clusters; the particle shows erosion on the surface due to knock-on radiation. This journal is © The Royal Society of Chemistry 2020 Nanoscale Advances Fig. 6a is approximately 7 106 electrons per A2. In the measurements performed using the TEM mode, we considered the electron dose frame per second (fps) or fractions of seconds (usually 0.5 fps), which is relatively low speed compared with ultra-fast acquisition.32 In the STEM mode, the parameter that is used to control the electron dose is the dwell time, which is the time in which the electron beam is retained per pixel. In the STEM mode, there is a compromise between the dwell time and electron dose used to study a few atoms in a cluster with atomic resolution. When the knock on is signicant the surface of the nanoparticle looks irregular and some atoms are dispersed outside the clusters, as shown in Fig. 6e. The damage produced by the emission of the Auger electrons can be signicant. The Auger eﬀect is produced by the lling of inner atomic shell vacancies by an electron in higher energy levels. The excess of energy is transfer to an outer shell electron, which is then emitted out of the atoms. The energy of the Auger electron can be released on the cluster or nanoparticle in the form of heat, this eﬀect was analyzed by Williams33 to explain the shape uctuations on the nanoparticles. Let us consider an Auger ionization event in a gold cluster. Every event produces 2 keV with a range of approximately 1.5 nm, which deposits approximately 0.3–0.4 eV per atom. For instance, if the electron dose is 104 electrons per Å2 per second in the Au144 cluster, 72 Auger events per second are generated. This will deliver 22.5 eV in the cluster every second. The clusters are placed on a carbon grid for observation in the TEM. As the ligand is an insulator there will be an increase in temperature on the cluster inducing radiation damage. For bigger nanoparticles, without the presence of ligands, part of the heat will be released to the substrate and the eﬀect will be negligible. Diﬀraction methods in STEM mode Selected area electron diﬀraction (SAED) is the most common method used to study the structure of materials. The reections used for the analysis of SAED patterns that are inside the zero order Laue zone (ZOLZ) are not suﬃcient to extract the 3D structural information of a crystal and therefore several zone axes must be registered. However, under certain modes of optical congurations in the microscope (a large convergence angle and large camera length), it is possible to obtain information on reections at the rst-order, second-order, third order, and so on, which are known collectively as the higherorder Laue zones (HOLZ). The information in the HOLZ regions is commonly used for studying symmetry in crystallography.34,35 For clusters and nanoparticles, an electron beam conned as a nanoprobe can also be used to obtain diﬀraction patterns from individual nanoparticles and it can be combined with a scanning process in the STEM mode. In this process, the scanning is stopped to register the diﬀraction pattern of the selected nanoparticle. The switching process between STEM and diﬀraction is dened as the D-STEM method. When the electron probe is stopped in a cluster, the diﬀraction pattern can be recorded using the charge-coupled device (CCD) camera. Under this conguration, the lateral resolution in real space is reduced; however, the image of the cluster is still clear enough Nanoscale Adv. View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Nanoscale Advances Fig. 7 Experimental and simulated examples of diﬀraction patterns using STEM mode. (a) An atomic model of a pentagonal nanoparticle, (b) a HAADF-STEM image of a pentagonal particle, indicating the position of the beam to extract the diﬀraction patterns with (c) a large convergence angle and (d) after the modiﬁcation of the values of the corrector lens (quasi-parallel illumination). The simulation of the electron diﬀraction patterns under nanobeam diﬀraction are shown below: (e) the simulation of the diﬀraction pattern using a semiconvergence angle of 3 mrad and (f) the diﬀraction pattern simulated with an angle of 0.5 mrad. Atomic models of the simulated patterns indicate the simulated probe size interacting with the nanoparticle. to identify the cluster or nanoparticle. Using aberrationcorrected microscopes with the probe corrector, it is possible to reduce the convergence angle and separate the convergent disks to reections when the beam is aligned in a quasi-parallel illumination. Electron diﬀraction patterns on the STEM patterns are obtained by positioning the beam in the STEM image using the Digiscan control, the scan is stopped in a region of interest and subsequently the pattern is recorded using a CCD camera. Fig. 7 shows diﬀraction patterns in the STEM mode under two diﬀerent semi-convergence angles. The semi-convergence angle is directly associated with the probe size, at large convergence angles the convergent beam electron diﬀraction (CBED) disks are formed. The D-STEM mode generates CBED patterns, which are adjusted to obtain diﬀraction patterns with spots instead of modifying the condenser lens excitation value and the excitation voltage of the adaptor lenses (ADL) of the hexapole of a corrected electron optical system (CEOS) corrector. In this process, the beam is aligned by the beam tilt and beam shi deectors. Fig. 7a shows the model of the pentagonal nanoparticle used in Fig. 7b, collected using a large convergence angle (Fig. 7c) and aer the separation and reduction of the disks, the reections are obtained (see Fig. 7d). The decahedron was used for practical purposes to illustrate the change from the large to the low convergence angle without deterioration of the sample. The consequence of the compensation can be simulated in a pentagonal particle (Fig. 7a) oriented near the zone axis of the experimental particle. The conditions for the simulations are a semi-convergence angle of 3 mrad (Fig. 7e), which is reduced to 0.5 mrad for quasi-parallel illumination, as shown in Fig. 7f. Simulations were performed using the java electron microscopy soware package.36 Under these illumination conditions, the electron beam is not precisely a convergent beam, but a quasiparallel illumination, in which the electron path is forced to Nanoscale Adv. Review Fig. 8 An Au144SR(60) cluster recorded using (a) a HAADF-STEM image23 (FFT image shown in (b)) and (c) a simulated image (with the simulated diﬀraction pattern shown in (d)), and (e) the HAADF-STEM image adjusted via (f) D-STEM. a localized area in the nanometric scale with a parallel illumination at the same time. For protected metallic clusters the electron beam irradiation is more critical owing to the high sensitivity of the ligands. To avoid damage, faster dwell times are employed before collection of the diﬀraction patterns. Fig. 8 shows a set of images to elucidate the structure of the cluster Au144SR(60). Fig. 8a shows a probe-corrected HAADF-STEM image and Fig. 8b shows the fast Fourier transform (FFT). Fig. 8c shows a simulated image of the metallic cluster (using simulaTEM37) and its diﬀraction pattern (Fig. 8d). Fig. 8e shows the HAADF-STEM image aer adjustments for D-STEM, as shown in Fig. 8f. The position of the beam from which the diﬀraction pattern is obtained is indicated in Fig. 8e. The diﬀraction pattern was collected under quasi-parallel illumination. The analysis of the diﬀraction patterns and atomic resolution images provides structural characterization of the individual metallic clusters. A novel perspective on the diﬀraction methods used under the STEM mode has been recently demonstrated using cryo-electron ptychography,28 which has been employed for sensitive materials for low-dose phase retrieval. Ptychography is an interesting method, in which electron microscopy is explored either in the real space or reciprocal space. In real space, ptychography is analogous to oﬀ-axis electron holography, one of the complementary methods used for phase retrieval and applied to sensitive specimens.27,29,38 Unlike the two alternative diﬀraction methods, electron and neutron diﬀraction, the analyses of electron diﬀraction are carried out in isolated clusters or nanoparticles, which makes the challenge more important given the high intensity of the electrons and the dynamic scattering, as previously explained. Similar to the two alternate techniques, data collection must be acquired in a few seconds or a fraction of a second. Even when the development of electron detectors is one step behind with respect to X-rays it is clear to see the complexity of identifying a single cluster owing to the multiple variables and the problem becomes analogous to the many body problem, not because we need to detect individual electrons that have deviated from the specimen, but the information from the wavefunction to the This journal is © The Royal Society of Chemistry 2020 View Article Online Review Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. exit of the sample and the use of probabilistic methods is prevalent. Crystal orientation mapping assisted with precession electron diﬀraction Precession electron diﬀraction (PED) has been used to reduce dynamical scattering, as proved and theoretically supported by Paul Midgley and Roger Vincent.16,17,39,40 The conical oscillation of the electron beam (performed between 50 and 100 Hz) is produced by scanning the deection of the scanning coils in the microscope. The method has been used to quantify the intensities for crystalline structure determination and also to enhance the electron energy loss spectroscopy (EELS)41 signal by compensating for channeling-induction.42,43 The reections excited during the precession process satisfy the Bragg condition at each moment, making the dynamical eﬀects less pronounced in the diﬀraction pattern. The intensities obtained are proportional to the square of the structure factor and the forbidden reections are signicantly reduced. Increasing the precession angle will make the Ewald sphere touch more points in the reciprocal space and more diﬀraction spots will be displayed in the diﬀraction pattern. Fig. 9a shows a STEM image of a polycrystalline YAG:Er sample, which was prepared using a focused ion beam (FIB), the inset shows the crystalline model generated using VESTA.22 Fig. 9b and c shows the experimental results; the electron diﬀraction patterns with precession oﬀ and on oriented along the h113i zone axis, respectively. The evidence of the enhancement of the reections is clear when the precession is activated. Fig. 9d shows the simulated electron diﬀraction pattern at a low camera length to show the zero and rst order Laue zones (FOLZ) as seen in the experimental pattern shown in Fig. 9b. The diﬀraction pattern simulated and shown in Fig. 9e was obtained without precession and for Nanoscale Advances a 50 nm electron-transparent thickness. Fig. 9f shows the simulated PED pattern with 1 of the precession angle, the experimental precession pattern corresponds to the quasikinematical case of the simulated pattern. Simulations were performed using the JEMS soware package.34,36 The diﬀraction pattern of Fig. 9d was obtained with the double-diﬀraction activation in the JEMS program, which plots the kinematically forbidden reections. A systematic indexing and crystal orientation mapping applied to TEM has been developed41,44 and combined with precession electron diﬀraction. This technique has become a useful tool to obtain crystal orientations and phase maps in relative short times.45 The principle consists of forming a small probe to be scanned through the area of interest on the sample, obtaining and recording an electron diﬀraction pattern at each step of the scanned area with an ultrafast (200 fps) external CCD camera. Every acquired electron diﬀraction pattern is stored in a computer to be later compared to pre-calculated templates; the diﬀraction pattern is indexed using cross-correlation to select the best match. The indexing result of the whole set of diﬀraction patterns can then be displayed as a phase or an orientation map of the scanned area.46 When using precession, the eﬀective focused beam size on the specimen will suﬀer from beam broadening owing to spherical aberration for the nonaxial trajectories, and this will be more noticeable when increasing the precession angle. At the end, the spatial resolution of the orientation/phase map will depend on the eﬀective beam size and on the scanning step chosen. On the other hand, the angular resolution obtained in the orientation maps will depend on the angular grid used for the generation of the templates. As the spot diﬀraction patterns are not sensitive to crystal tilts of less than 1 , values are usually given between 0.5 and 1 . Though there is the possibility of selecting a smaller sample value by increasing the number of generated templates so that between a given template and the closest one there is 0.2–0.5 .44 To avoid duplicities in the orientation assignation it is necessary to use precession angles lower than 1 . This must be taken into consideration when choosing the precession angle for phase or orientation mapping. Hence, the crystal orientation and phase mapping consist of two main steps: the fast acquisitions of spot patterns and the reliable orientation identication. This brings the necessity of additional hardware equipment that must be used with the microscope and soware to carry out the analysis. The degree of matching between an experimental diﬀraction pattern and a calculated one is given by the following equation:44 m P P xj ; yj Ti xj ; yj j¼1 QðiÞ ¼ sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃsﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ m m P P P2 xj ; yj Ti 2 xk ; yj (a) An STEM image of a YAG:Er polycrystalline sample; (b) a low camera length SAED pattern of an individual grain oriented along the h113i zone axis. (c) An experimental PED pattern collected at 1 in the same zone axis. (d) A simulated electron diﬀraction pattern at low camera length with double diﬀraction; (e) a simulated electron diﬀraction pattern without precession and with 50 nm of electrontransparent thickness; and (f) a simulated PED pattern at 1 for comparison with the experimental case. Fig. 9 This journal is © The Royal Society of Chemistry 2020 j¼1 j¼1 In which, the pattern is represented by the intensity function P(x,y) while every template i is given by the function Ti(x,y). The highest Q value corresponds to the solution. In this way, the quality of the pattern matching can be evaluated by the assigned Nanoscale Adv. View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Nanoscale Advances Fig. 10 A schematic representation of the virtual bright ﬁeld recon- struction. A virtual aperture is used to select only the transmitted beam and this is then plotted on the image. This is equivalent to introducing an aperture in the beam path (adapted with permission from ref. 47). pixel values of the index maps. Additionally, a reliability index value is determined between the two highest optimum solutions Q1 and Q2 of the matching: R ¼ 100(1 Q2/Q1). A reliability index value will be low when more than one orientation or phase is contained in a diﬀraction spot pattern. This value is assigned to each pixel corresponding to an indexed diﬀraction pattern, in this way a reliability map can be generated. A lower value will correspond to a darker pixel and a higher value will correspond to a brighter pixel. The range will depend on the maximum reliability value calculated. To reconstruct a bright eld image of the object, the average intensity is calculated in a disc that surrounds the transmitted beam from the recorded diﬀraction pattern (Fig. 10). The inner part of the transmitted beam saturates, leaving the contrast information in the outer part. Therefore, the virtual aperture needs to be larger than the transmitted beam. In this virtual bright eld STEM mode, it is the beam diameter that delimits the virtual bright eld image resolution.46 In a similar way, the virtual aperture may be displaced on one of the spots of the diﬀraction pattern and form a virtual dark eld image. An example of the crystal orientation mapping is shown in Fig. 11 in which the gold pentagonal nanoparticle is orientated along the observation axis z (zone axis). The orientation map with respect to z is colored in green, showing an orientation of  for the whole nanoparticle. The index map shows dark areas along the twin boundaries of the particle owing to the double spot feature in the diﬀraction pattern. This is also observed in the reliability map along the twin boundaries of the Review Fig. 12 (a) Crystal orientation mapping of a set of particles observed along the z-axis; (b) a virtual bright ﬁeld image; (c) a correlation map showing twin planes, where the particles indicated by arrows do not show twins; and (d) the color key for the cubic crystal orientation map.49 nanoparticle. In Fig. 11e–g, the orientation maps have been combined with the index map, and this feature allows the twin boundaries to be distinguished. Crystal orientation maps, with respect to x and y, show a degree of rotation between each tetrahedron, two pairs of them have a similar orientation. The PED pattern acquisition conditions were as follows: NBD mode with a 0.8 nm spot size, 20 mm aperture, precession angle of 0.5 at 50 Hz, and scanning with a step size of 1 nm. Structural defects such as grain boundaries, dislocations and twins can be visualized by using correlation coeﬃcient mapping, which consists of computing the diﬀerences between neighboring diﬀraction patterns in the scanned area of the scanning electron diﬀraction patterns.48 A set of particles has been used to highlight the presence of twin boundaries. In Fig. 12 the crystal orientation map of regular polyhedral particles is shown, as well as its virtual bright eld image (Fig. 12b). The corresponding correlation contour maps clearly exhibit the inner contrasts that correspond to the multiple twin boundaries contained within the nanoparticles. In contrast, for nontwinned particles contours appear only at the edges of the particle and there is no contrast in the center of the nanoparticles marked with arrows in Fig. 12c. This evidence has been used to eliminate the possibility of twins in the  direction, cutting the particle into two. To reconstruct a virtual bright-eld image from the diﬀraction patterns, a virtual aperture is placed over the transmitted beam of the recorded diﬀraction patterns. Then, the average intensity is calculated leaving out the contrast information from the diﬀraction spots. In this sense the image formed is a STEM type bright-eld image of the object. Coherent electron diﬀraction of nanoparticles Fig. 11 (a) A TEM micrograph of a gold nanoparticle (the color key for the cubic crystal orientation map is shown in the inset). (b) A virtual bright ﬁeld image, (c) index map, (d) reliability map, (e) crystal orientation map with respect to the z-axis, (f) crystal orientation map with respect to the y-axis, and (g) crystal orientation map with respect to the x-axis. Nanoscale Adv. One of the most useful methods used to study nanoparticles is the use of diﬀraction using a parallel coherent electron beam, as shown by Zuo and Spence.50 By adjusting the condenser lenses (illumination) it is possible, by good approximation, to assume that the beam is a point source and the electron probe is coherent. This is dened by the coherent length L. If the nanoparticle size R is greater than or equal to L, then the diﬀraction pattern will show rods of intensity. From the directions of the rods in reciprocal space we can determine the miller indexes of the facets. This journal is © The Royal Society of Chemistry 2020 View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Review Fig. 13 (A) A TEM image of a rectangular evaporated gold nanoparticle.51 (A0 ) A coherent electron diﬀraction pattern using a 40 nm beam probe to cover the particle and produce streaks in the reﬂections (B) A scanning electron micrograph with its respective EDS mapping for (Ag) silver and (Au) gold, and crystal orientation mapping in the three axes, x, y, z, of the pentagonal [email protected] particle. (B0 ) A coherent electron diﬀraction pattern using a 660 nm beam probe to cover the particle and produce streaks in the reﬂections; the TEM micrograph is shown in the inset. We present two examples of gold nanoparticles: a rectangular particle obtained by thermal evaporation (Fig. 13A)51 and a pentagonal shape (Fig. 13B) with multiple facets in the surface.52 The streaks on the diﬀraction patterns are directly related to the crystallography of the facets.53 The probe diameter used for the rectangular particle was set to 40 nm. The pentagonal is very large and in order to obtain a complete diﬀraction pattern a probe size of 660 nm was used. This gives an example of the electron diﬀraction used to identify surface faceting in nanoparticles. In both cases the nanoprobe illumination with a quasi-parallel illumination produces the coherent diﬀraction patterns of each particle. Nanoscale Advances possibility of structural renement; and (ii) the phase of the reections cannot be extracted directly from the electron diﬀraction pattern. Accuracy depends largely on the electrontransparent thickness of the specimen; if the sample is thick, the diﬀraction becomes more dynamic and this reduces the information at reections further away from the transmitted beam. The reduction of the reections in the reciprocal space limits the scattering vector Q, related to the atomic scattering factor as Q ¼ (4p sin q)/l, which results in a reduction of the resolution in real space. One of the best methodologies used to extract the structure of the crystal, short-range order and amorphous materials is the atomic pair distribution function (PDF). PDF is an extraordinary technique in diﬀraction physics for studying the nanostructure of crystals using highly energetic neutron or synchrotron X-ray sources. The two diﬀraction methods have demonstrated a high reliability to elucidate the structure of materials, while electron diﬀraction (ePDF) has been used to a lesser extent owing to the high inelastic scattering within the crystals. The PDF g(r) is the probability of nding the nearest neighbor at an interatomic distance of r.54 SAED patterns of randomly oriented particles dispersed on a carbon thin lm are used as a traditional method to study the structure of crystals. The rings in the diﬀraction patterns are correlated to a family of planes of the crystal and analysis is straightforward. One of the advantages of using electron diﬀraction is that one can collect the diﬀraction pattern from a single nanoparticle. However, using the SAED patterns in the ePDF method is less accurate than the other two diﬀraction methods owing to the high dynamic scattering.55 However, the use of PED and low temperatures (liquid nitrogen) reduces the dynamic contribution and the thermal scattering, respectively. The result of the PED-ePDF improvement is the enhancement of the intensities for a higher scattering vector Q.56,57 The example shown in the HRTEM image shown in Fig. 14a corresponds to lipoic acid ligand-protected gold nanoparticles with an average size of 4.5 nm.58 The SAED pattern shown in Fig. 14b was recorded using a CMOS TVIPS camera 16 bit grayscale, this includes over 65 000 shades of gray, and an electron dose of approximately 35 electrons per A2. The azimuthal intensity Electron pair distribution functions in metallic clusters The irradiation of materials with electrons in a TEM is an alternated process that goes from real to reciprocal space. An image recorded at high resolution or lattice resolution, is usually postprocessed from the real space to the Fourier space. However, from an electron diﬀraction pattern the opposite process is not a direct process for two main reasons: (i) the high dynamic scattering within the sample produces forbidden reections with very strong intensities which disable the This journal is © The Royal Society of Chemistry 2020 Fig. 14 (a) A HRTEM image of a set of gold nanoparticles, (b) an SAED pattern collected at low temperature; (c) a simulated PDF of an fcc gold structure; and extracted ePDFs (d) without precession and (e) with precession. Nanoscale Adv. View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Nanoscale Advances prole is in the inset of the SAED pattern shown in Fig. 14b. Fig. 14c shows the calculated PDF of an fcc gold structure using the OVITO soware package.59 The distances of the rst nearest neighbors are not aﬀected by the size of the particle; only by an increase in the number of peaks for bigger particles. The number of neighbors is directly related to the coordination numbers of the particle. The experimental set up was a combination of the precession unit manufactured by Nanomegas and the low temperature using a cold stage. The precession was operated at 100 Hz and a precession angle of 2 . The azimuthal intensity prole was extracted using DiﬀTools V5 (ref. 60) in a digital micrograph. The pair distribution function of the sample is shown in Fig. 14d (no precession) and Fig. 14e (precession activated) and these were extracted using the SUePDF program.61 The ePDFs are compared with the theoretical PDF and it is noticeable that an improvement in the precession ePDF is observed at the second nearest neighbor and the last two peaks in the g(r). The example shown in Fig. 14 demonstrates the eﬀectiveness of ePDF on the metallic nanoparticles, but so far, the internal structure that could be aﬀected by structural defects is not measured and we cannot quantify how accurate the measurement is. The next step is quantitative comparison with diﬀerent types of particles, regular fcc and multiply twinned domains. We have considered three diﬀerent cases, which were identied in the HRTEM images: the icosahedron (Ih) (Fig. 15a), truncated octahedron (TOh) (Fig. 15b) and decahedron (Dh) (Fig. 15c). The models of these structures have been simulated using a pythonbased code,62 and jmol soware was used for visualization.63 Cluster structure models were built for the case of clusters with Ih symmetry with 2869 atoms, clusters with a truncated fcc symmetry with the shape of an octahedron (TOh) with 2899 atoms, and clusters with decagonal symmetry (Dh) with 2869 atoms. For the truncated octahedron model using the Wulﬀ construction, the surface potentials were used, as detailed in a previous publication.64 In this analysis, the subtraction of the amorphous carbon lm (free of nanoparticles) was applied by collecting electron diﬀraction patterns of a set of particles and the carbon lm (10 nm). Both diﬀraction patterns, carbon lm Fig. 15 HRTEM images of the identiﬁed NPs: (a) Ih, (b) TOh, and (c) Dh and the corresponding structural models used. PDF ﬁt analysis in comparison with diﬀerent structural models: (a0 ) Ih, Rw 36%, (b0 ) TOh, Rw 24%, and (c0 ) Dh, Rw 22% (adapted from ref. 56 with permission). Nanoscale Adv. Review and nanoparticles, were captured under the same illumination conditions (area of diﬀraction, camera length, precession, and electron dose). The tting between experimental and simulated PDF functions was performed using DiﬀPy-CMI, a python-based program.65 Fig. 15a0 –c0 shows the ePDF t analysis using these three structures and the diﬀerences. The tting provides a percentage error between the models and experimental ePDFs that is measured by the least-square residuum Rw (residual error),66 which were measured as Ih, Rw 36%, TOh, Rw 24%, and Dh, Rw 22%. The high Q region may contain information that is dominated by noise. The truncation of the experimental data produces ripples, especially around strong peaks; these unphysical peaks can be easily misinterpreted as extra structural features. The t range and Qmax used in all the diﬀraction patterns were 2–15 (Å), and 20 (Å1), respectively. Cryogenic conditions (liquid N2) resulted in an intensity prole that contains more signals at a higher Q. Resolution damping (Qdamp) and the atomic displacement parameter are two quantities that improved from the precession being oﬀ to the precession being turned on.56 The results obtained herein using the improved PED are comparable with the results obtained using high energy X-ray sources.67 An article published by Banerjee et al. demonstrated the evaluation of X-ray PDF data applied to metallic nanoparticles by using the cluster-mining approach.68 In this approach, the residual error is adjusted through a cluster-screen map with the structure models of the nanoparticles and their maximum number of atoms, which results in a generalized methodology to determine the structures rather than the individual tting of experimental data and the possible structural motifs. This approach can be implemented for low electron dose illumination and liquid nitrogen temperature conditions to obtain the ePDF and applied to ligand-protected metallic clusters, in which singularity in the properties is directly related to the crystalline structure. Data analytics to decouple nanoscale materials and related crystallographic chemistry In order to address the probabilistic problem for crystal determination, the starting point is that the crystal momentum is conserved, and images or diﬀraction patterns collected from damaged samples will be not considered or will be used for another batch with diﬀerent structures. The simplest case is the static beam and static sample, shown in the scheme in Fig. 16a, which can be used for more than one particle that is oriented diﬀerently. The dynamic electron beam is when the scanning mode is applied (Fig. 16b) and the sample or the set of samples remains in their original positions, the beam position is displaced to the coordinates (xi, yj) in the space in two-dimensions owing to the projected image in the plate of the camera. However, even when the clusters are deposited in a at area, such as carbon lm, they are represented by 3D crystal models. For a metallic cluster we have previously found that the probe size must be in the range of the particle size, ideally less to This journal is © The Royal Society of Chemistry 2020 View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Review Fig. 16 Various schematic diagrams relating to the collection of diﬀraction patterns of metallic clusters under nanobeam diﬀraction: (a) when the beam and the clusters are static; (b) when the nanobeam is scanned over the sample, but the sample is stable, and (c) when the sample and electron beam are dynamic and a large data set of electron diﬀraction patterns in the same area is necessary. obtain isolated patterns, and a high lateral resolution is crucial. When the samples are dynamic, it means that the specimen can rotate owing to the momentum generated by the electrons,69 then a new variable is added, and the need for a fast detector becomes important to improve the temporal resolution (Fig. 16c). In this way, the signal-to-noise-ratio increases, and the analysis become more complicated. In order to process the large data set of electron diﬀraction patterns, algorithm-powered, human-guided data exploration and characterization creates a powerful symbiosis between researchers and their tools. The breadth of data collected simultaneously in the latest generation of STEM is useful for exploring nanoparticles and their intrinsic subtleties presents opportunities for advancing synthesis and model development. Enabling these advances is the ability to explore high spatial, temporal, and energetic domains. This includes imaging, diﬀraction, and spectroscopy in the exploration, development, and integration of these tools with multimodal data analytics and the statistics associated with many machine and deep learning approaches. Natively, this includes compressive, regressive, and classication routines that enable researchers to go beyond data collection and burdensome post data analysis into near-autonomous automation and materials-informed process control. Arguably, the most useful information gained using STEM is identifying the structure of the underlying materials, including specic atomic arrangements and relationships, derived from high-resolution imaging, spectroscopy, and diﬀraction-based techniques. Beyond single imaging, spectroscopy, or advanced diﬀraction methods, precession-based electron diﬀraction, compressive imaging, and multidimensional imaging, for example, four-dimensional microscopy, have emerged to extend the capability for combined analytical work.70–77 These same methods have led to the expressed urgency for translating crystallographic information and deviations from massive datasets in support of basic and applied materials challenges. With a propensity to generate large datasets addressing data proliferation amongst all these platforms, it is paramount to guide the synthesis, and underlying strategies for harvesting This journal is © The Royal Society of Chemistry 2020 Nanoscale Advances highly functionalized nanoparticles are critical. The breadth of simultaneously collected data in the latest generation of scanning transmission electron microscopes presents numerous opportunities for expanding the collective eﬃciency, and the analysis of nanostructured, and conned material systems.78–80 The native resolution of many modern microscopes varies within each microscope from approximately 0.50 to over 2 angstroms. Recent advances leveraging deep learning have made it possible to analyze human-intractable diﬀraction datasets and perform complex imaging tasks, including segmentation and classication.81 This includes various material systems ranging from conventional metals and oxides to resolving the chemical evolution at complex interfaces and junctions.82 However, deep learning and augmented analysis for decoupling nanoscale eﬀects have not yet disrupted the performance of classifying and segmenting data from either highly temporally or spatially resolved datasets obtained upon the advent of four-dimensional microscopy. In practical terms, four-dimensional microscopy is not limited by the native resolution of the microscope, but rather the ability to relay and process information in the context of materials science. Researchers have addressed multimodal microscopy from diﬀraction-focused techniques based on separating the elastic and inelastic portions associated with fundamental scattering. In Fig. 17, each pixel represents a single electron diﬀraction pattern, containing both central elastic and inelastic portions, in which reections are located at the (x,y) position of the reciprocal space and each pattern is collected at another (x0 ,y0 ) position in the region of the analysis, as shown in the diﬀraction patterns shown in Fig. 17. Fig. 18 represents a smaller multidimensional diﬀraction dataset, in which the model developed by Aguiar et al. is used to convert each pattern into a crystal family prediction at each pixel. The strength associated with each prediction is reported without a priori or ab initio-based knowledge.83,84 By processing each pattern, the probability and prominence between crystal families reects the underlying structural changes at each hyper pixel, between the presence of a nanoparticle and the underlying grid. Isolating areas prominently containing the particle Fig. 17 Multidimensional microscopy data for collecting high-reso- lution diﬀraction patterns and underlying proﬁles. Over the space, each frame presents a single electron diﬀraction pattern containing both the elastic and inelastic portions of electron scattering, allowing for separating the components of the elastic and inelastic portions. Nanoscale Adv. View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Nanoscale Advances Fig. 18 Detailed crystal chemistry analysis of multidimensional microscopy data. (a) Applying the convolutional neural network-based crystal model by Aguiar et al. we report the overall crystallographic family classiﬁcation per pixel using up to six peaks for each diﬀraction pattern. Without a priori knowledge, the calculated per pixel classiﬁcation provides an underlying crystal family level prediction, reporting the most prominent phase. Following this overarching classiﬁcation, the underlying predictions for the crystal family are supported by points and, eventually, space groups based on selecting the two super pixels that are outlined in purple and green. Comparing the pixels, both (b) cubic and trigonal families are strongly predicted, and the all cubic families in (c) highlight the predictive and hierarchical model nature. At the lowest granularity for the space group, each of these previous plotted distributions provides the prominence of the primary cubic and trigonal components based on the underlying space groups, respectively, for each family. and the grid, Fig. 18b and c reect the underlying predicted space group distribution for cubic and trigonal, in which each of these are the primary components in the hyper pixelated diﬀraction dataset. It should be further noted that based on the predictive crystal model from the electron diﬀraction patterns alone can be extended to larger datasets, including for example in Fig. 19a, in which identifying the underlying family, point, and space group distribution is required at this scale. It should be noted that each sub-pixelated electron diﬀraction pattern exemplied in Fig. 19b is classied for 3 to 6 peak combinations, forming a distribution and multiple predictions per point. With an expressed need to quickly evaluate the data, the model translates each pattern in Fig. 19c into a prediction for the crystal family, point group, and space group. This follows the ability to translate data as shown in Fig. 19d over specic pixels, rows, or columns, as congured by the user. The data reported here are only simple examples of the many potential Nanoscale Adv. Review Extension to large diﬀraction datasets. (a) Via extension, the method can be applied over larger datasets including more than the (b) individual patterns collected over a larger imaging space. (c) Based on the predictions for each diﬀraction pattern, a classiﬁcation map for the crystal family, point group, or prominent space group can be calculated; in this case, a crystal family is reported. (d) Beyond single pixels, the analysis can be performed over rows or columns. Note that the space group is reported for each column aligned with the prior family classiﬁcation. Fig. 19 avenues for which the model has been applied and now provides a larger community with a predictive and scalable tool for translating raw structural data from either high-resolution atomic-scale images or diﬀraction into predictive structural phase information, not limited by specic models or prior expertise. Leveraging the advances to develop a computer vision and articial intelligence engine for translating crystallographic and structural data now presents the opportunity for automation and augmentation of synthesis and control over nanostructured and nanoscale materials. Deep-learning models such as the one reported, have now been developed to circumvent classication, segmentation, and compression challenges. A limited number of these machine or deep-learning models have been proposed and have demonstrated sub-image sampling in image segmentation and inpainting over the fast to slow temporal This journal is © The Royal Society of Chemistry 2020 View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Review regimes, allowing adaptive event tracking and augmentation over current microscope imaging, diﬀraction, and spectroscopic feeds. The main application being in situ microscopy, in which studying processes such as self-assembly, molecular organization, and catalysis, can be improved by the development of improved physics-based models by eliminating superuous assumptions. Our temporal understanding associated with these processes is limited to a holistic understanding that is tied to the underlying fundamentals, including the eﬀects of temperature, solution supersaturation, interfacial kinetics, and activation potential. The barrier to independent crystallographic structural determination has mainly been addressed. Now, the challenge is in translating the body of materials knowledge from the current databases into advanced and adaptive physics-informed workows that are not limited to high-resolution electron microscopes and diﬀractometers used to study the nanoscale phenomenon. Conclusions Electron diﬀraction methods applied to materials in the sizeranges of tens or hundreds of nanometers have been used for several decades to characterize the crystalline structures of solids. This review presents advanced methods of electron diﬀraction that can be applied to metallic clusters (few nanometers) and nanoparticles. The complementary methods of characterization for metallic clusters and particles that are used to measure their properties are linked to their sizes, shapes, and crystalline structures. In this review we have discussed advanced methods of electron diﬀraction, emphasizing the signicant potential of this technique. Most of our examples have involved Au clusters; however, the methods are equally valid for other metals and their alloys. Electron diﬀraction methods relating to TEM are still being developed. The main challenge for the future is to reduce the acquisition time and, therefore, the radiation damage to the cluster; it is particularly important to assure the integrity of the capping ligand. If the capping ligand is damaged, the cluster will become unstable and atomic rearrangements can occur that will alter the results. One possible improvement will be to pulse the beam to reduce the residence time. Additionally, large data sets are required to improve structural analysis. This eld therefore still faces challenges, but the future is bright. Conﬂicts of interest All authors declare that they have no competing interests. Acknowledgements AP gratefully acknowledges nancial support provided by the Department of Defense W911NF-18-1-0439 as well as the VPREDKE-T2 project at UTSA. This work was partially funded by MIRA -NAU with a seed grant. J. A. A. and J. T. performed the diﬀraction analysis, contributed gures, draed the section on data analytics, and reviewed the entire manuscript. The authors acknowledge several contributors for providing samples for This journal is © The Royal Society of Chemistry 2020 Nanoscale Advances analysis: D. Sanchez, P. Parajuli, R. Mendoza, M. Hoque, J. J. Velazquez-Salazar, S. Vergara, A. Dass, and P. Horta. References 1 P. Chakraborty, A. Nag, A. Chakraborty and T. Pradeep, Acc. Chem. Res., 2019, 52, 2–11. 2 T. Higaki, Y. Li, S. Zhao, Q. Li, S. Li, X.-S. Du, S. Yang, J. Chai and R. Jin, Angew. Chem., Int. Ed., 2019, 58, 8291–8302. 3 E. A. Doud, A. Voevodin, T. J. Hochuli, A. M. Champsaur, C. Nuckolls and X. Roy, Nat. Rev. Mater., 2020, 5, 371–387. 4 A. Dass, J. Am. Chem. Soc., 2011, 133, 19259–19261. 5 F. Baletto and R. Ferrando, Rev. Mod. Phys., 2005, 77, 371– 423. 6 R. Jin, Nanoscale, 2015, 7, 1549–1565. 7 J. Yang and R. Jin, ACS Mater. Lett., 2019, 1, 482–489. 8 X. Kang and M. Zhu, Chem. Soc. Rev., 2019, 48, 2422–2457. 9 Q. Tang, G. Hu, V. Fung and D.-e. Jiang, Acc. Chem. Res., 2018, 51, 2793–2802. 10 Y. Watanabe, Sci. Technol. Adv. Mater., 2014, 15, 063501. 11 P. D. Jadzinsky, G. Calero, C. J. Ackerson, D. A. Bushnell and R. D. Kornberg, Science, 2007, 318, 430–433. 12 M. W. Heaven, A. Dass, P. S. White, K. M. Holt and R. W. Murray, J. Am. Chem. Soc., 2008, 130, 3754–3755. 13 N. K. Chaki, Y. Negishi, H. Tsunoyama, Y. Shichibu and T. Tsukuda, J. Am. Chem. Soc., 2008, 130, 8608–8610. 14 K. M. Harkness, Y. Tang, A. Dass, J. Pan, N. Kothalawala, V. J. Reddy, D. E. Cliﬀel, B. Demeler, F. Stellacci, O. M. Bakr and J. A. McLean, Nanoscale, 2012, 4, 4269–4274. 15 D. B. Williams and C. B. Carter, Transmission Electron Microscopy, Springer US, 2009. 16 A. Avilov, K. Kuligin, S. Nicolopoulos, M. Nickolskiy, K. Boulahya, J. Portillo, G. Lepeshov, B. Sobolev, J. P. Collette, N. Martin, A. C. Robins and P. Fischione, Ultramicroscopy, 2007, 107, 431–444. 17 S. Nicolopoulos, A. Kuligin, K. Kuligin, B. Khalid, G. Lepeshov, J. L. DelPlancke, A. Avilov, M. Nickolsky and A. Ponce, Electron Crystallography: Novel Approaches for Structure Determination of Nanosized Materials, 2006, vol. 211, pp. 169–280. 18 S. Vergara, U. Santiago, C. Kumara, D. Alducin, R. L. Whetten, M. J. Yacaman, A. Dass and A. Ponce, J. Phys. Chem. C, 2018, 122, 26733–26738. 19 S. Vergara, D. A. Lukes, M. W. Martynowycz, U. Santiago, G. Plascencia-Villa, S. C. Weiss, M. J. de la Cruz, D. M. Black, M. M. Alvarez, X. López-Lozano, C. O. Barnes, G. Lin, H.-C. Weissker, R. L. Whetten, T. Gonen, M. J. Yacaman and G. Calero, J. Phys. Chem. Lett., 2017, 8, 5523–5530. 20 S. Iijima and T. Ichihashi, Phys. Rev. Lett., 1986, 56, 616–619. 21 R. F. Egerton, P. Li and M. Malac, Micron, 2004, 35, 399–409. 22 K. Momma and F. Izumi, J. Appl. Crystallogr., 2011, 44, 1272– 1276. 23 D. Bahena, N. Bhattarai, U. Santiago, A. Tlahuice, A. Ponce, S. B. H. Bach, B. Yoon, R. L. Whetten, U. Landman and M. Jose-Yacaman, J. Phys. Chem. Lett., 2013, 4, 975–981. 24 R. F. Egerton, Ultramicroscopy, 2013, 127, 100–108. Nanoscale Adv. View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Nanoscale Advances 25 G. McMullan, A. T. Clark, R. Turchetta and A. R. Faruqi, Ultramicroscopy, 2009, 109, 1411–1416. 26 D. Weber, A. Clausen and R. E. Dunin-Borkowski, in Handbook on Big Data and Machine Learning in the Physical Sciences, 2018, pp. 83–120, DOI: 10.1142/ 9789811204579_0005. 27 E. Voelkl, R. Herring, B. Bammes and D. Hoyle, Microsc. Microanal., 2015, 21, 1951–1952. 28 L. Zhou, J. Song, J. S. Kim, X. Pei, C. Huang, M. Boyce, L. Mendonça, D. Clare, A. Siebert, C. S. Allen, E. Liberti, D. Stuart, X. Pan, P. D. Nellist, P. Zhang, A. I. Kirkland and P. Wang, Nat. Commun., 2020, 11, 2773. 29 L. J. Shery Chang, J. Barthel, R. Dunin-Borkowski and C. Dwyer, in European Microscopy Congress 2016: Proceedings, 2016, pp. 769–770, DOI: 10.1002/ 9783527808465.Emc2016.6971. 30 J. P. Buban, Q. Ramasse, B. Gipson, N. D. Browning and H. Stahlberg, J. Electron Microsc., 2010, 59, 103–112. 31 E. Ortega, A. Ponce, U. Santiago, D. Alducin, A. Benitez-Lara, G. Plascencia-Villa and M. Jose-Yacaman, Adv. Struct. Chem. Imaging, 2016, 2, 22–27. 32 A. Mittelberger, C. Kramberger and J. C. Meyer, Ultramicroscopy, 2018, 188, 1–7. 33 P. Williams, Appl. Phys. Lett., 1987, 50, 1760–1762. 34 J. P. Mornirolli, P. Stadelmann, G. Ji and S. Nicolopoulos, J. Microsc., 2010, 237, 511–515. 35 J. P. Morniroli, G. Ji and D. Jacob, Ultramicroscopy, 2012, 121, 42–60. 36 P. A. Stadelmann, Ultramicroscopy, 1987, 21, 131–145. 37 A. Gómez-Rodrı́guez, L. M. Beltrán-del-Rı́o and R. HerreraBecerra, Ultramicroscopy, 2010, 110, 95–104. 38 E. Voelkl and A. Ponce, Microsc. Microanal., 2018, 24, 1462– 1463. 39 R. Vincent and P. A. Midgley, Ultramicroscopy, 1994, 53, 271– 282. 40 M. Blackman and G. P. Thomson, Proc. R. Soc. London, Ser. A, 1939, 173, 68–82. 41 E. F. Rauch and M. Véron, Microsc. Microanal., 2016, 22, 500– 501. 42 P. P. Das, S. Nicolopoulos and M. Gemmi, Acta Crystallogr., Sect. A: Found. Adv., 2017, 73, C983. 43 L. Yedra, P. Torruella, A. Eljarrat, A. D. Darbal, J. K. Weiss, F. Peiró and S. Estradé, Appl. Phys. Lett., 2014, 105, 053117. 44 E. F. Rauch and M. Véron, Mater. Charact., 2014, 98, 1–9. 45 D. Viladot, M. Veron, M. Gemmi, F. Peiró, J. Portillo, S. Estradé, J. Mendoza, N. Llorca-Isern and S. Nicolopoulos, J. Microsc., 2013, 252, 23–34. 46 E. F. Rauch and M. Veron, Materialwiss. Werkstoech., 2005, 36, 552–556. 47 F. Ruiz-Zepeda, D. Bahena, A. Ponce and D. I. GarciaGutierrez, in Advanced Transmission Electron Microscopy, ed. L. F. Deepak, M. Alcala and R. Arenal, Springer, Cham, 2015, ch. 2, DOI: 10.1007/978-3-319-15177-9_2. 48 Á. K. Kiss, E. F. Rauch and J. L. Lábár, Ultramicroscopy, 2016, 163, 31–37. 49 U. Santiago, J. J. Velazquez-Salazar, J. E. Sanchez, F. RuizZepeda, J. E. Ortega, J. Reyes-Gasga, L. Bazan-Diaz, Nanoscale Adv. Review 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65 66 67 68 I. Betancourt, E. F. Rauch, M. Veron, A. Ponce and M. JoseYacaman, Surf. Sci., 2016, 644, 80–85. J. M. Zuo and J. C. H. Spence, Advanced Transmission Electron Microscopy, Springer, New York, NY, 2017. R. Mendoza-Cruz, D. Romeu, L. Bazan-Diaz, J. Enrique Samaniego, U. Santiago, A. Ponce and M. Jose-Yacaman, Cryst. Growth Des., 2017, 17, 6062–6070. U. Santiago, J. J. Velázquez-Salazar, J. E. Sanchez, F. RuizZepeda, J. E. Ortega, J. Reyes-Gasga, L. Bazán-Dı́az, I. Betancourt, E. F. Rauch, M. Veron, A. Ponce and M. JoséYacamán, Surf. Sci., 2016, 644, 80–85. A. B. Shah, S. T. Sivapalan, B. M. DeVetter, T. K. Yang, J. Wen, R. Bhargava, C. J. Murphy and J.-M. Zuo, Nano Lett., 2013, 13, 1840–1846. S. J. L. Billinge, J. Solid State Chem., 2008, 181, 1695–1700. C. L. Farrow and S. J. L. Billinge, Acta Crystallogr., Sect. A: Found. Crystallogr., 2009, 65, 232–239. M. M. Hoque, S. Vergara, P. P. Das, D. Ugarte, U. Santiago, C. Kumara, R. L. Whetten, A. Dass and A. Ponce, J. Phys. Chem. C, 2019, 123, 19894–19902. C. Fernando, M. M. Hoque, J. Reyes Gasga and A. Ponce, Microsc. Microanal., 2019, 25, 1926–1927. M. M. Hoque, K. M. Mayer, A. Ponce, M. M. Alvarez and R. L. Whetten, Langmuir, 2019, 35, 10610–10617. A. Stukowski, Modell. Simul. Mater. Sci. Eng., 2009, 18, 015012. D. R. G. Mitchell, Microsc. Res. Tech., 2008, 71, 588–593. D. T. Tran, G. Svensson and C.-W. Tai, J. Appl. Crystallogr., 2017, 50, 304–312. A. Hjorth Larsen, J. Jørgen Mortensen, J. Blomqvist, I. E. Castelli, R. Christensen, M. Dułak, J. Friis, M. N. Groves, B. Hammer, C. Hargus, E. D. Hermes, P. C. Jennings, P. Bjerre Jensen, J. Kermode, J. R. Kitchin, E. Leonhard Kolsbjerg, J. Kubal, K. Kaasbjerg, S. Lysgaard, J. Bergmann Maronsson, T. Maxson, T. Olsen, L. Pastewka, A. Peterson, C. Rostgaard, J. Schiøtz, O. Schütt, M. Strange, K. S. Thygesen, T. Vegge, L. Vilhelmsen, M. Walter, Z. Zeng and K. W. Jacobsen, J. Phys.: Condens. Matter, 2017, 29, 273002. Jmol: an open-source Java viewer for chemical structures in 3D, http://www.jmol.org/. J.-M. Zhang, F. Ma and K.-W. Xu, Appl. Surf. Sci., 2004, 229, 34–42. P. Juhas, C. L. Farrow, X. Yang, K. R. Knox and S. J. L. Billinge, Acta Crystallogr., Sect. A: Found. Adv., 2015, 71, 562–568. S. Banerjee, C.-H. Liu, J. D. Lee, A. Kovyakh, V. Grasmik, O. Prymak, C. Koenigsmann, H. Liu, L. Wang, A. M. M. Abeykoon, S. S. Wong, M. Epple, C. B. Murray and S. J. L. Billinge, J. Phys. Chem. C, 2018, 122, 29498–29506. K. M. Ø. Jensen, P. Juhas, M. A. Tofanelli, C. L. Heinecke, G. Vaughan, C. J. Ackerson and S. J. L. Billinge, Nat. Commun., 2016, 7, 11859. S. Banerjee, C.-H. Liu, K. M. O. Jensen, P. Juhas, J. D. Lee, M. Tofanelli, C. J. Ackerson, C. B. Murray and S. J. L. Billinge, Acta Crystallogr., Sect. A: Found. Adv., 2020, 76, 24–31. This journal is © The Royal Society of Chemistry 2020 View Article Online Open Access Article. Published on 16 November 2020. Downloaded on 1/10/2021 6:18:04 AM. This article is licensed under a Creative Commons Attribution-NonCommercial 3.0 Unported Licence. Review 69 L. D. Marks and J. P. Zhang, Ultramicroscopy, 1992, 41, 419– 422. 70 S. Jesse, B. J. Rodriguez, S. Choudhury, A. P. Baddorf, I. Vrejoiu, D. Hesse, M. Alexe, E. A. Eliseev, A. N. Morozovska, J. Zhang, L.-Q. Chen and S. V. Kalinin, Nat. Mater., 2008, 7, 209–215. 71 S. Jesse and S. V. Kalinin, Nanotechnology, 2009, 20, 085714. 72 T. LaGrange, G. H. Campbell, J. D. Colvin, B. Reed and W. E. King, J. Mater. Sci., 2006, 41, 4440–4444. 73 M. S. Grinolds, V. A. Lobastov, J. Weissenrieder and A. H. Zewail, Proc. Natl. Acad. Sci. U. S. A., 2006, 103, 18427–18431. 74 V. A. Lobastov, R. Srinivasan and A. H. Zewail, Proc. Natl. Acad. Sci. U. S. A., 2005, 102, 7069–7073. 75 R. M. v. d. Veen, T. J. Penfold and A. H. Zewail, Struct. Dyn., 2015, 2, 024302. 76 A. Yurtsever and A. H. Zewail, Proc. Natl. Acad. Sci. U. S. A., 2011, 108, 3152–3156. This journal is © The Royal Society of Chemistry 2020 Nanoscale Advances 77 A. H. Zewail, Science, 2010, 328, 187–193. 78 P. D. Nellist and S. J. Pennycook , Scanning Transmission Electron Microscopy, Springer-Verlag New York, 2011. 79 N. Dellby, L. Krivanek, D. Nellist, E. Batson and R. Lupini, J. Electron Microsc., 2001, 50, 177–185. 80 J. M. LeBeau, S. D. Findlay, L. J. Allen and S. Stemmer, Phys. Rev. Lett., 2008, 100, 206101. 81 W. Li, K. G. Field and D. Morgan, npj Comput. Mater., 2018, 4, 36. 82 F. Cappia, B. D. Miller, J. A. Aguiar, L. He, D. J. Murray, B. J. Frickey, J. D. Stanek and J. M. Harp, J. Nucl. Mater., 2020, 531, 151964. 83 J. A. Aguiar, M. L. Gong, R. R. Unocic, T. Tasdizen and B. D. Miller, Sci. Adv., 2019, 5, eaaw1949. 84 J. A. Aguiar, M. L. Gong and T. Tasdizen, Comput. Mater. Sci., 2020, 173, 109409. Nanoscale Adv.